Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- NORMA Astm a 653_galvanizado ZINC by pedroluis_choque 639 views
- Welding of clad plates: Recommended... by labeebmlp 1567 views
- Is2062.2006 by guest03ca43c 23449 views
- Steel engineer handbook by Hoang Thang 3352 views
- Heat_exchanger_mechanical_design_ca... by MIGUEL SALDIVAR H... 550 views
- Stress-Strain Curve by Ghulam Mehdi 321 views

3,218 views

3,033 views

3,033 views

Published on

No Downloads

Total views

3,218

On SlideShare

0

From Embeds

0

Number of Embeds

21

Shares

0

Downloads

80

Comments

0

Likes

2

No embeds

No notes for slide

- 1. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. Section 5 Strength of Materials BY JOHN SYMONDS Fellow Engineer (Retired), Oceanic Division, Westinghouse Electric Corporation. J. P. VIDOSIC Regents’ Professor Emeritus of Mechanical Engineering, Georgia Institute of Technology. Late Manager, Product Standards and Services, Columbus McKinnon Corporation, Tonawanda, N.Y. DONALD D. DODGE Supervisor (Retired), Product Quality and Inspection Technology, Manufacturing Development, Ford Motor Company. HAROLD V. HAWKINS 5.1 MECHANICAL PROPERTIES OF MATERIALS by John Symonds, Expanded by Staff Stress-Strain Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-2 Fracture at Low Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-7 Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-8 Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-10 Hardness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-12 Testing of Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-13 5.2 MECHANICS OF MATERIALS by J. P. Vidosic Simple Stresses and Strains . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-15 Combined Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-18 Plastic Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-19 Design Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-20 Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-20 Torsion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-36 Columns . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-38 Eccentric Loads . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-40 Curved Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-41 Impact . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-43 Theory of Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-44 Cylinders and Spheres . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-45 Pressure between Bodies with Curved Surfaces . . . . . . . . . . . . . . . . . . . . . . 5-47 Flat Plates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-47 Theories of Failure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-48 Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-49 Rotating Disks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-50 Experimental Stress Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-51 5.3 PIPELINE FLEXURE STRESSES by Harold V. Hawkins Pipeline Flexure Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-55 5.4 NONDESTRUCTIVE TESTING by Donald D. Dodge Nondestructive Testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-61 Magnetic Particle Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-61 Penetrant Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-61 Radiographic Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-65 Ultrasonic Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-66 Eddy Current Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-66 Microwave Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-67 Infrared Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-67 Acoustic Signature Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5-67 5-1
- 2. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5.1 MECHANICAL PROPERTIES OF MATERIALS by John Symonds, Expanded by Staff REFERENCES: Davis et al., ‘‘Testing and Inspection of Engineering Materials,’’ McGraw-Hill, Timoshenko, ‘‘Strength of Materials,’’ pt . II, Van Nostrand. Richards, ‘‘Engineering Materials Science,’’ Wadsworth. Nadai, ‘‘Plasticity,’’ McGraw-Hill. Tetelman and McEvily, ‘‘Fracture of Structural Materials,’’ Wiley. ‘‘Fracture Mechanics,’’ ASTM STP-833. McClintock and Argon (eds.), ‘‘Mechanical Behavior of Materials,’’ Addison-Wesley. Dieter, ‘‘Mechanical Metallurgy,’’ McGraw-Hill. ‘‘Creep Data,’’ ASME. ASTM Standards, ASTM. Blaznynski (ed.), ‘‘Plasticity and Modern Metal Forming Technology,’’ Elsevier Science. permanent strain. The permanent strain commonly used is 0.20 percent of the original gage length. The intersection of this line with the curve determines the stress value called the yield strength. In reporting the yield strength, the amount of permanent set should be speciﬁed. The arbitrary yield strength is used especially for those materials not exhibiting a natural yield point such as nonferrous metals; but it is not limited to these. Plastic behavior is somewhat time-dependent, particularly at high temperatures. Also at high temperatures, a small amount of time-dependent reversible strain may be detectable, indicative of anelastic behavior. STRESS-STRAIN DIAGRAMS The Stress-Strain Curve The engineering tensile stress-strain curve is obtained by static loading of a standard specimen, that is, by applying the load slowly enough that all parts of the specimen are in equilibrium at any instant. The curve is usually obtained by controlling the loading rate in the tensile machine. ASTM Standards require a loading rate not exceeding 100,000 lb/in2 (70 kgf/mm2)/min. An alternate method of obtaining the curve is to specify the strain rate as the independent variable, in which case the loading rate is continuously adjusted to maintain the required strain rate. A strain rate of 0.05 in/in/(min) is commonly used. It is measured usually by an extensometer attached to the gage length of the specimen. Figure 5.1.1 shows several stress-strain curves. Fig. 5.1.2. Fig. 5.1.1. Comparative stress-strain diagrams. (1) Soft brass; (2) low carbon steel; (3) hard bronze; (4) cold rolled steel; (5) medium carbon steel, annealed; (6) medium carbon steel, heat treated. For most engineering materials, the curve will have an initial linear elastic region (Fig. 5.1.2) in which deformation is reversible and timeindependent. The slope in this region is Young’s modulus E. The proportional elastic limit (PEL) is the point where the curve starts to deviate from a straight line. The elastic limit (frequently indistinguishable from PEL) is the point on the curve beyond which plastic deformation is present after release of the load. If the stress is increased further, the stress-strain curve departs more and more from the straight line. Unloading the specimen at point X (Fig. 5.1.2), the portion XXЈ is linear and is essentially parallel to the original line OXЈЈ. The horizontal distance OXЈ is called the permanent set corresponding to the stress at X. This is the basis for the construction of the arbitrary yield strength. To determine the yield strength, a straight line XXЈ is drawn parallel to the initial elastic line OXЈЈ but displaced from it by an arbitrary value of 5-2 General stress-strain diagram. The ultimate tensile strength (UTS) is the maximum load sustained by the specimen divided by the original specimen cross-sectional area. The percent elongation at failure is the plastic extension of the specimen at failure expressed as (the change in original gage length ϫ 100) divided by the original gage length. This extension is the sum of the uniform and nonuniform elongations. The uniform elongation is that which occurs prior to the UTS. It has an unequivocal signiﬁcance, being associated with uniaxial stress, whereas the nonuniform elongation which occurs during localized extension (necking) is associated with triaxial stress. The nonuniform elongation will depend on geometry, particularly the ratio of specimen gage length L 0 to diameter D or square root of crosssectional area A. ASTM Standards specify test-specimen geometry for a number of specimen sizes. The ratio L 0 /√A is maintained at 4.5 for ﬂatand round-cross-section specimens. The original gage length should always be stated in reporting elongation values. The specimen percent reduction in area (RA) is the contraction in cross-sectional area at the fracture expressed as a percentage of the original area. It is obtained by measurement of the cross section of the broken specimen at the fracture location. The RA along with the load at fracture can be used to obtain the fracture stress, that is, fracture load divided by cross-sectional area at the fracture. See Table 5.1.1. The type of fracture in tension gives some indications of the quality of the material, but this is considerably affected by the testing temperature, speed of testing, the shape and size of the test piece, and other conditions. Contraction is greatest in tough and ductile materials and least in brittle materials. In general, fractures are either of the shear or of the separation (loss of cohesion) type. Flat tensile specimens of ductile metals often show shear failures if the ratio of width to thickness is greater than 6 : 1. A completely shear-type failure may terminate in a chisel edge, for a ﬂat specimen, or a point rupture, for a round specimen. Separation failures occur in brittle materials, such as certain cast irons. Combinations of both shear and separation failures are common on round specimens of ductile metal. Failure often starts at the axis in a necked region and produces a relatively ﬂat area which grows until the material shears along a cone-shaped surface at the outside of the speci-
- 3. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. STRESS-STRAIN DIAGRAMS 5-3 Table 5.1.1 Typical Mechanical Properties at Room Temperature (Based on ordinary stress-strain values) Metal Tensile strength, 1,000 lb/in 2 Yield strength, 1,000 lb/in 2 Ultimate elongation, % Reduction of area, % Brinell no. Cast iron Wrought iron Commercially pure iron, annealed Hot-rolled Cold-rolled Structural steel, ordinary Low-alloy, high-strength Steel, SAE 1300, annealed Quenched, drawn 1,300°F Drawn 1,000°F Drawn 700°F Drawn 400°F Steel, SAE 4340, annealed Quenched, drawn 1,300°F Drawn 1,000°F Drawn 700°F Drawn 400°F Cold-rolled steel, SAE 1112 Stainless steel, 18-S Steel castings, heat-treated Aluminum, pure, rolled Aluminum-copper alloys, cast Wrought , heat-treated Aluminum die castings Aluminum alloy 17ST Aluminum alloy 51ST Copper, annealed Copper, hard-drawn Brasses, various Phosphor bronze Tobin bronze, rolled Magnesium alloys, various Monel 400, Ni-Cu alloy Molybdenum, rolled Silver, cast , annealed Titanium 6 – 4 alloy, annealed Ductile iron, grade 80-55-06 18 – 60 45 – 55 42 48 100 50 – 65 65 – 90 70 100 130 200 240 80 130 190 240 290 84 85 – 95 60 – 125 13 – 24 19 – 23 30 – 60 30 56 48 32 68 40 – 120 40 – 130 63 21 – 45 79 100 18 130 80 8 – 40 25 – 35 19 30 95 30 – 40 40 – 80 40 80 110 180 210 45 110 170 215 260 76 30 – 35 30 – 90 5 – 21 12 – 16 10 – 50 0 35 – 25 48 30 0 55 – 30 85 75 100 – 300 100 70 90 200 120 150 150 200 260 400 480 170 270 395 480 580 160 145 – 160 120 – 250 23 – 44 50 – 80 50 – 120 40 – 30 30 – 15 26 24 20 14 10 25 20 14 12 10 18 60 – 55 33 – 14 35 – 5 4–0 33 – 15 2 26 20 58 4 60 – 3 55 – 5 40 17 – 0.5 48 30 54 10 6 34 40 5 60 8 – 80 41 11 – 30 30 75 8 120 55 70 – 40 70 65 60 45 30 70 60 50 48 44 45 75 – 65 65 – 20 39 35 73 55 52 75 25 100 105 45 100 50 – 170 50 – 200 120 47 – 78 125 250 27 352 225 – 255 NOTE: Compressive strength of cast iron, 80,000 to 150,000 lb/in 2. Compressive yield strength of all metals, except those cold-worked ϭ tensile yield strength. Stress 1,000 lb/in 2 ϫ 6.894 ϭ stress, MN/m 2. men, resulting in what is known as the cup-and-cone fracture. Double cup-and-cone and rosette fractures sometimes occur. Several types of tensile fractures are shown in Fig. 5.1.3. Annealed or hot-rolled mild steels generally exhibit a yield point (see Fig. 5.1.4). Here, in a constant strain-rate test, a large increment of extension occurs under constant load at the elastic limit or at a stress just below the elastic limit. In the latter event the stress drops suddenly from the upper yield point to the lower yield point. Subsequent to the drop, the yield-point extension occurs at constant stress, followed by a rise to the UTS. Plastic ﬂow during the yield-point extension is discontinuous; Fig. 5.1.3. to test temperature, test strain rate, and the characteristics of the tensile machine employed. The plastic behavior in a uniaxial tensile test can be represented as the true stress-strain curve. The true stress is based on the instantaneous Typical metal fractures in tension. successive zones of plastic deformation, known as Luder’s bands or stretcher strains, appear until the entire specimen gage length has been uniformly deformed at the end of the yield-point extension. This behavior causes a banded or stepped appearance on the metal surface. The exact form of the stress-strain curve for this class of material is sensitive Fig. 5.1.4. Yielding of annealed steel.
- 4. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-4 MECHANICAL PROPERTIES OF MATERIALS cross section A, so that ϭ load/A. The instantaneous true strain increment is Ϫ dA/A, or dL/L prior to necking. Total true strain is ͵ A A0 Ϫ dA ϭ ln A ͩͪ A0 A or ln (L/L0 ) prior to necking. The true stress-strain curve or ﬂow curve obtained has the typical form shown in Fig. 5.1.5. In the part of the test subsequent to the maximum load point (UTS), when necking occurs, the true strain of interest is that which occurs in an inﬁnitesimal length at the region of minimum cross section. True strain for this element can still be expressed as ln (A0 /A), where A refers to the minimum cross section. Methods of constructing the true stress-strain curve are described in the technical literature. In the range between initial yielding and the neighborhood of the maximum load point the relationship between plastic strain p and true stress often approximates ϭ kn p where k is the strength coefﬁcient and n is the work-hardening exponent. For a material which shows a yield point the relationship applies only to the rising part of the curve beyond the lower yield. It can be shown that at the maximum load point the slope of the true stress-strain curve equals the true stress, from which it can be deduced that for a material obeying the above exponential relationship between p and n, p ϭ n at the maximum load point. The exponent strongly inﬂuences the spread between YS and UTS on the engineering stress-strain curve. Values of n and k for some materials are shown in Table 5.1.2. A point on the ﬂow curve indentiﬁes the ﬂow stress corresponding to a certain strain, that is, the stress required to bring about this amount of plastic deformation. The concept of true strain is useful for accurately describing large amounts of plastic deformation. The linear strain deﬁnition (L Ϫ L 0 )/L 0 fails to correct for the continuously changing gage length, which leads to an increasing error as deformation proceeds. During extension of a specimen under tension, the change in the specimen cross-sectional area is related to the elongation by Poisson’s ratio , which is the ratio of strain in a transverse direction to that in the longitudinal direction. Values of for the elastic region are shown in Table 5.1.3. For plastic strain it is approximately 0.5. Table 5.1.2 Room-Temperature Plastic-Flow Constants for a Number of Metals Material 0.40% C steel 0.05% C steel 2024 aluminum 2024 aluminum Copper 70 – 30 brass Fig. 5.1.5. True stress-strain curve for 20°C annealed mild steel. k, 1,000 in 2 (MN/m 2) 0.088 72 (49.6) 100 (689) 49 (338) 46.4 (319) 130 (895) Quenched and tempered at 400°F (478K) Annealed and temper-rolled Precipitation-hardened Annealed Annealed Annealed n 416 (2,860) Condition 0.235 0.16 0.21 0.54 0.49 SOURCE: Reproduced by permission from ‘‘Properties of Metals in Materials Engineering,’’ ASM, 1949. Table 5.1.3 Elastic Constants of Metals (Mostly from tests of R. W. Vose) Metal E Modulus of elasticity (Young’s modulus). 1,000,000 lb/in 2 G Modulus of rigidity (shearing modulus). 1,000,000 lb/in2 Cast steel Cold-rolled steel Stainless steel 18 – 8 All other steels, including high-carbon, heat-treated Cast iron Malleable iron Copper Brass, 70 – 30 Cast brass Tobin bronze Phosphor bronze Aluminum alloys, various Monel metal Inconel Z-nickel Beryllium copper Elektron (magnesium alloy) Titanium (99.0 Ti), annealed bar Zirconium, crystal bar Molybdenum, arc-cast 28.5 29.5 27.6 28.6 – 30.0 13.5 – 21.0 23.6 15.6 15.9 14.5 13.8 15.9 9.9 – 10.3 25.0 31 30 17 6.3 15 – 16 11 – 14 48 – 52 11.3 11.5 10.6 11.0 – 11.9 5.2 – 8.2 9.3 5.8 6.0 5.3 5.1 5.9 3.7 – 3.9 9.5 11 11 7 2.5 6.5 K Bulk modulus. 1,000,000 lb/in 2 Poisson’s ratio 20.2 23.1 23.6 22.6 – 24.0 8.4 – 15.5 17.2 17.9 15.7 16.8 16.3 17.8 9.9 – 10.2 22.5 4.8 0.265 0.287 0.305 0.283 – 0.292 0.211 – 0.299 0.271 0.355 0.331 0.357 0.359 0.350 0.330 – 0.334 0.315 0.27 – 0.38 Ϯ 0.36 Ϯ 0.21 0.281 0.34
- 5. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. STRESS-STRAIN DIAGRAMS /2 2r d /2 D ؉ r ؉ III 1)2 ϭ 2(ys r d r Stress concentration factor, K 3.4 3.0 2.6 I IV 2.2 II 1.8 III V 1.4 Note; in all cases Dϭdϩ2r 1.0 0.01 0.1 0.2 1.0 r d Fig. 5.1.6. Flat plate with semicircular ﬁllets and grooves or with holes. I, II, and III are in tension or compression; IV and V are in bending. ؉ r D )2 Stress-strain curves in the plastic region for combined stress loading can be constructed. However, a particular stress state does not determine a unique strain value. The latter will depend on the stress-state path which is followed. Plane strain is a condition where strain is conﬁned to two dimensions. There is generally stress in the third direction, but because of mechanical constraints, strain in this dimension is prevented. Plane strain occurs in certain metalworking operations. It can also occur in the neighborhood of a crack tip in a tensile loaded member if the member is sufﬁciently thick. The material at the crack tip is then in triaxial tension, which condition promotes brittle fracture. On the other hand, ductility is enhanced and fracture is suppressed by triaxial compression. Stress Concentration In a structure or machine part having a notch or any abrupt change in cross section, the maximum stress will occur at this location and will be greater than the stress calculated by elementary formulas based upon simpliﬁed assumptions as to the stress distribution. The ratio of this maximum stress to the nominal stress (calculated by the elementary formulas) is the stress-concentration factor Kt . This is a constant for the particular geometry and is independent of the material, provided it is isotropic. The stress-concentration factor may be determined experimentally or, in some cases, theoretically from the mathematical theory of elasticity. The factors shown in Figs. 5.1.6 to 5.1.13 were determined from both photoelastic tests and the theory of elasticity. Stress concentration will cause failure of brittle materials if d r D h d h r 3.4 Stress concentration factor, K ϩ (2 Ϫ 3 ϩ (2 Ϫ )2 r D ؉ (1 Ϫ 2 )2 ؉ V d 1 Ϫ 3 ϭ ys in which 1 and 3 are the largest and smallest principal stresses, respectively, and ys is the uniaxial tensile yield strength. This is the simplest theory for predicting yielding under combined stresses. A more accurate prediction can be made by the distortion-energy theory, according to which the criterion is d r II r D r D For most engineering materials at room temperature the strain rate sensitivity is of the order of 0.01. The effect becomes more signiﬁcant at elevated temperatures, with values ranging to 0.2 and sometimes higher. Compression Testing The compressive stress-strain curve is similar to the tensile stress-strain curve up to the yield strength. Thereafter, the progressively increasing specimen cross section causes the compressive stress-strain curve to diverge from the tensile curve. Some ductile metals will not fail in the compression test. Complex behavior occurs when the direction of stressing is changed, because of the Bauschinger effect, which can be described as follows: If a specimen is ﬁrst plastically strained in tension, its yield stress in compression is reduced and vice versa. Combined Stresses This refers to the situation in which stresses are present on each of the faces of a cubic element of the material. For a given cube orientation the applied stresses may include shear stresses over the cube faces as well as stresses normal to them. By a suitable rotation of axes the problem can be simpliﬁed: applied stresses on the new cubic element are equivalent to three mutually orthogonal principal stresses 1 , 2 , 3 alone, each acting normal to a cube face. Combined stress behavior in the elastic range is described in Sec. 5.2, Mechanics of Materials. Prediction of the conditions under which plastic yielding will occur under combined stresses can be made with the help of several empirical theories. In the maximum-shear-stress theory the criterion for yielding is that yielding will occur when ؉ IV d ؉ ͪ I ؉ ͩ Bending ؉ mϭ ␦ log ␦ log Tension or compression ؉ The general effect of increased strain rate is to increase the resistance to plastic deformation and thus to raise the ﬂow curve. Decreasing test temperature also raises the ﬂow curve. The effect of strain rate is expressed as strain-rate sensitivity m. Its value can be measured in the tension test if the strain rate is suddenly increased by a small increment during the plastic extension. The ﬂow stress will then jump to a higher value. The strain-rate sensitivity is the ratio of incremental changes of log and log 5-5 3.0 2.6 2.2 h ϭ d Semi-circle grooves (hϭr) Blunt grooves 02 0. 05 0. 1 0. 2 0. Sharp grooves 5 0. 1 1.8 2 1.4 1.0 0.4 1.0 1.5 2 h Sharpness of groove, r Fig. 5.1.7. Flat plate with grooves, in tension. 3 4 5 6
- 6. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. MECHANICAL PROPERTIES OF MATERIALS ؉ r the concentrated stress is larger than the ultimate strength of the material. In ductile materials, concentrated stresses higher than the yield strength will generally cause local plastic deformation and redistribution of stresses (rendering them more uniform). On the other hand, even with ductile materials areas of stress concentration are possible sites for fatigue if the component is cyclically loaded. h d h D r ؉ r d h D ؉ 02 05 0. 1 0. fill 2.6 of Blunt fillets 5 0. 02 h d ϭ Blunt fillets Sharp fillets 1.8 0.5 1 1.0 1.5 2 3 4 5 6 h Sharpness of fillet, r Fig. 5.1.10. Flat plate with ﬁllets, in bending. 0.5 Sharp fillets 2 1.0 0.4 0.2 th 2.2 2.2 2 0. 1.4 0. ϭ h d ϭ Dϭd ϩ 2h Full fillets (hϭr) et 3.0 De p Stress concentration factor, K 3.4 Dϭd ϩ 2h Full fillets (hϭr) 2.6 1 h 3.0 0. ؉ r Stress concentration factor, K 3.4 0 .0 5-6 1.0 1.8 2.0 1.4 1.0 0.4 1.0 1.5 2 3 4 5 6 h Sharpness of fillet, r Fig. 5.1.8. Flat plate with ﬁllets, in tension. Flat plate with angular notch, in tension or bending. ؉ r ؉ r D h d h r ؉ 5 5 0.2 Sharp grooves 1.8 1 2 1.4 3.0 Semi circ. grooves hϭr 1 Stress concentration factor, K 0.1 0.0 d ϭ 2.2 0. 2.6 Dϭd ϩ 2h Semi-circle grooves (hϭr) h Stress concentration factor, K 3.0 D h d ϭ 0. 1 3.4 3.4 h d 0.4 Fig. 5.1.11. 2.6 2.2 Blunt grooves 1.8 Sharp grooves h ϭ 0.04 d 4 1.4 10 1.0 0.4 1.0 1.5 2 Sharpness of groove, Fig. 5.1.9. Flat plate with grooves, in bending. 3 4 5 6 1.0 0.5 h r 1.0 1.5 2 3 4 5 6 Sharpness of groove, Fig. 5.1.12. Grooved shaft in torsion. 8 10 h r 15 20
- 7. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. FRACTURE AT LOW STRESSES D ؉ r h d h ϭ 0.05 d 3.0 Dϭd ϩ 2h Full fillets (hϭr) 2.6 0.1 Sharp fillets 2.2 5 0. Blunt fillets 1.8 0. 2 Stress concentration factor, K 3.4 1 1.4 1.0 0.5 1.0 2 3 4 5 7 10 20 40 h Sharpness of fillet, r Fig. 5.1.13. Filleted shaft in torsion. FRACTURE AT LOW STRESSES Materials under tension sometimes fail by rapid fracture at stresses much below their strength level as determined in tests on carefully prepared specimens. These brittle, unstable, or catastrophic failures originate at preexisting stress-concentrating ﬂaws which may be inherent in a material. The transition-temperature approach is often used to ensure fracturesafe design in structural-grade steels. These materials exhibit a characteristic temperature, known as the ductile brittle transition (DBT) temperature, below which they are susceptible to brittle fracture. The transition-temperature approach to fracture-safe design ensures that the 5-7 transition temperature of a material selected for a particular application is suitably matched to its intended use temperature. The DBT can be detected by plotting certain measurements from tensile or impact tests against temperature. Usually the transition to brittle behavior is complex, being neither fully ductile nor fully brittle. The range may extend over 200°F (110 K) interval. The nil-ductility temperature (NDT), determined by the drop weight test (see ASTM Standards), is an important reference point in the transition range. When NDT for a particular steel is known, temperature-stress combinations can be speciﬁed which deﬁne the limiting conditions under which catastrophic fracture can occur. In the Charpy V-notch (CVN) impact test, a notched-bar specimen (Fig. 5.1.26) is used which is loaded in bending (see ASTM Standards). The energy absorbed from a swinging pendulum in fracturing the specimen is measured. The pendulum strikes the specimen at 16 to 19 ft (4.88 to 5.80 m)/s so that the specimen deformation associated with fracture occurs at a rapid strain rate. This ensures a conservative measure of toughness, since in some materials, toughness is reduced by high strain rates. A CVN impact energy vs. temperature curve is shown in Fig. 5.1.14, which also shows the transitions as given by percent brittle fracture and by percent lateral expansion. The CVN energy has no analytical signiﬁcance. The test is useful mainly as a guide to the fracture behavior of a material for which an empirical correlation has been established between impact energy and some rigorous fracture criterion. For a particular grade of steel the CVN curve can be correlated with NDT. (See ASME Boiler and Pressure Vessel Code.) Fracture Mechanics This analytical method is used for ultra-highstrength alloys, transition-temperature materials below the DBT temperature, and some low-strength materials in heavy section thickness. Fracture mechanics theory deals with crack extension where plastic effects are negligible or conﬁned to a small region around the crack tip. The present discussion is concerned with a through-thickness crack in a tension-loaded plate (Fig. 5.1.15) which is large enough so that the crack-tip stress ﬁeld is not affected by the plate edges. Fracture mechanics theory states that unstable crack extension occurs when the work required for an increment of crack extension, namely, surface energy and energy consumed in local plastic deformation, is exceeded by the elastic-strain energy released at the crack tip. The elastic-stress Fig. 5.1.14. CVN transition curves. (Data from Westinghouse R & D Lab.)
- 8. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-8 MECHANICAL PROPERTIES OF MATERIALS ﬁeld surrounding one of the crack tips in Fig. 5.1.15 is characterized by the stress intensity KI, which has units of (lb √in) /in2 or (N√m) /m 2. It is a function of applied nominal stress , crack half-length a, and a geometry factor Q: K 2 ϭ Q 2 a l (5.1.1) for the situation of Fig. 5.1.15. For a particular material it is found that as KI is increased, a value Kc is reached at which unstable crack propa- Table 5.1.4 Materials* Room-Temperature K lc Values on High-Strength Material 0.2% YS, 1,000 in 2 (MN/m 2) K lc , 1,000 in 2 √in (MN m 1/2 /m 2) 18% Ni maraging steel 18% Ni maraging steel 18% Ni maraging steel Titanium 6-4 alloy Titanium 6-4 alloy Aluminum alloy 7075-T6 Aluminum alloy 7075-T6 300 (2,060) 270 (1,850) 198 (1,360) 152 (1,022) 140 (960) 75 (516) 64 (440) 46 (50.7) 71 (78) 87 (96) 39 (43) 75 (82.5) 26 (28.6) 30 (33) * Determined at Westinghouse Research Laboratories. crack, and loadings (Paris and Sih, ‘‘Stress Analysis of Cracks,’’ STP381, ASTM, 1965). Failure occurs in all cases when Kt reaches KIc . Fracture mechanics also provides a framework for predicting the occurrence of stress-corrosion cracking by using Eq. (5.1.2) with KIc replaced by KIscc , which is the material parameter denoting resistance to stresscorrosion-crack propagation in a particular medium. Two standard test specimens for KIc determination are speciﬁed in ASTM standards, which also detail specimen preparation and test procedure. Recent developments in fracture mechanics permit treatment of crack propagation in the ductile regime. (See ‘‘Elastic-Plastic Fracture,’’ ASTM.) Fig. 5.1.15. Through-thickness crack geometry. gation occurs. Kc depends on plate thickness B, as shown in Fig. 5.1.16. It attains a constant value when B is great enough to provide plane-strain conditions at the crack tip. The low plateau value of Kc is an important material property known as the plane-strain critical stress intensity or fracture toughness K Ic . Values for a number of materials are shown in Table 5.1.4. They are inﬂuenced strongly by processing and small changes in composition, so that the values shown are not necessarily typical. KIc can be used in the critical form of Eq. (5.1.1): (KIc )2 ϭ Q 2acr (5.1.2) to predict failure stress when a maximum ﬂaw size in the material is known or to determine maximum allowable ﬂaw size when the stress is set. The predictions will be accurate so long as plate thickness B satisﬁes the plane-strain criterion: B Ն 2.5(KIc/ys )2. They will be conservative if a plane-strain condition does not exist. A big advantage of the fracture mechanics approach is that stress intensity can be calculated by equations analogous to (5.1.1) for a wide variety of geometries, types of Fig. 5.1.16. Dependence of K c and fracture appearance (in terms of percentage of square fracture) on thickness of plate specimens. Based on data for aluminum 7075-T6. (From Scrawly and Brown, STP-381, ASTM.) FATIGUE Fatigue is generally understood as the gradual deterioration of a material which is subjected to repeated loads. In fatigue testing, a specimen is subjected to periodically varying constant-amplitude stresses by means of mechanical or magnetic devices. The applied stresses may alternate between equal positive and negative values, from zero to maximum positive or negative values, or between unequal positive and negative values. The most common loading is alternate tension and compression of equal numerical values obtained by rotating a smooth cylindrical specimen while under a bending load. A series of fatigue tests are made on a number of specimens of the material at different stress levels. The stress endured is then plotted against the number of cycles sustained. By choosing lower and lower stresses, a value may be found which will not produce failure, regardless of the number of applied cycles. This stress value is called the fatigue limit. The diagram is called the stress-cycle diagram or S-N diagram. Instead of recording the data on cartesian coordinates, either stress is plotted vs. the logarithm of the number of cycles (Fig. 5.1.17) or both stress and cycles are plotted to logarithmic scales. Both diagrams show a relatively sharp bend in the curve near the fatigue limit for ferrous metals. The fatigue limit may be established for most steels between 2 and 10 million cycles. Nonferrous metals usually show no clearly deﬁned fatigue limit. The S-N curves in these cases indicate a continuous decrease in stress values to several hundred million cycles, and both the stress value and the number of cycles sustained should be reported. See Table 5.1.5. The mean stress (the average of the maximum and minimum stress values for a cycle) has a pronounced inﬂuence on the stress range (the algebraic difference between the maximum and minimum stress values). Several empirical formulas and graphical methods such as the ‘‘modiﬁed Goodman diagram’’ have been developed to show the inﬂuence of the mean stress on the stress range for failure. A simple but conservative approach (see Soderberg, Working Stresses, Jour. Appl. Mech., 2, Sept. 1935) is to plot the variable stress Sv (one-half the stress range) as ordinate vs. the mean stress Sm as abscissa (Fig. 5.1.18). At zero mean stress, the ordinate is the fatigue limit under completely reversed stress. Yielding will occur if the mean stress exceeds the yield stress So , and this establishes the extreme right-hand point of the diagram. A straight line is drawn between these two points. The coordinates of any other point along this line are values of Sm and Sv which may produce failure. Surface defects, such as roughness or scratches, and notches or
- 9. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. FATIGUE 5-9 Accordingly, the pragmatic approach to arrive at a solution to a design problem often takes a conservative route and sets q ϭ 1. The exact material properties at play which are responsible for notch sensitivity are not clear. Further, notch sensitivity seems to be higher, and ordinary fatigue strength lower in large specimens, necessitating full-scale tests in many cases (see Peterson, Stress Concentration Phenomena in Fatigue of Fig. 5.1.18. Fig. 5.1.17. The S-N diagrams from fatigue tests. (1) 1.20% C steel, quenched and drawn at 860°F (460°C); (2) alloy structural steel; (3) SAE 1050, quenched and drawn at 1,200°F (649°C); (4) SAE 4130, normalized and annealed; (5) ordinary structural steel; (6) Duralumin; (7) copper, annealed; (8) cast iron (reversed bending). shoulders all reduce the fatigue strength of a part. With a notch of prescribed geometric form and known concentration factor, the reduction in strength is appreciably less than would be called for by the concentration factor itself, but the various metals differ widely in their susceptibility to the effect of roughness and concentrations, or notch sensitivity. For a given material subjected to a prescribed state of stress and type of loading, notch sensitivity can be viewed as the ability of that material to resist the concentration of stress incidental to the presence of a notch. Alternately, notch sensitivity can be taken as a measure of the degree to which the geometric stress concentration factor is reduced. An attempt is made to rationalize notch sensitivity through the equation q ϭ (Kf Ϫ 1)/(K Ϫ 1), where q is the notch sensitivity, K is the geometric stress concentration factor (from data similar to those in Figs. 5.1.5 to 5.1.13 and the like), and Kf is deﬁned as the ratio of the strength of unnotched material to the strength of notched material. Ratio Kf is obtained from laboratory tests, and K is deduced either theoretically or from laboratory tests, but both must reﬂect the same state of stress and type of loading. The value of q lies between 0 and 1, so that (1) if q ϭ 0, Kf ϭ 1 and the material is not notch-sensitive (soft metals such as copper, aluminum, and annealed low-strength steel); (2) if q ϭ 1, Kf ϭ K, the material is fully notch-sensitive and the full value of the geometric stress concentration factor is not diminished (hard, high-strength steel). In practice, q will lie somewhere between 0 and 1, but it may be hard to quantify. Table 5.1.5 Effect of mean stress on the variable stress for failure. Metals, Trans. ASME, 55, 1933, p. 157, and Buckwalter and Horger, Investigation of Fatigue Strength of Axles, Press Fits, Surface Rolling and Effect of Size, Trans. ASM, 25, Mar. 1937, p. 229). Corrosion and galling (due to rubbing of mating surfaces) cause great reduction of fatigue strengths, sometimes amounting to as much as 90 percent of the original endurance limit. Although any corroding agent will promote severe corrosion fatigue, there is so much difference between the effects of ‘‘sea water’’ or ‘‘tap water’’ from different localities that numerical values are not quoted here. Overstressing specimens above the fatigue limit for periods shorter than necessary to produce failure at that stress reduces the fatigue limit in a subsequent test. Similarly, understressing below the fatigue limit may increase it. Shot peening, nitriding, and cold work usually improve fatigue properties. No very good overall correlation exists between fatigue properties and any other mechanical property of a material. The best correlation is between the fatigue limit under completely reversed bending stress and the ordinary tensile strength. For many ferrous metals, the fatigue limit is approximately 0.40 to 0.60 times the tensile strength if the latter is below 200,000 lb/in2. Low-alloy high-yield-strength steels often show higher values than this. The fatigue limit for nonferrous metals is approximately to 0.20 to 0.50 times the tensile strength. The fatigue limit in reversed shear is approximately 0.57 times that in reversed bending. In some very important engineering situations components are cyclically stressed into the plastic range. Examples are thermal strains resulting from temperature oscillations and notched regions subjected to secondary stresses. Fatigue life in the plastic or ‘‘low-cycle’’ fatigue range has been found to be a function of plastic strain, and low-cycle fatigue testing is done with strain as the controlled variable rather than stress. Fatigue life N and cyclic plastic strain p tend to follow the relationship N2 ϭ C p where C is a constant for a material when N Ͻ 105. (See Cofﬁn, A Study Typical Approximate Fatigue Limits for Reversed Bending Metal Tensile strength, 1,000 lb/in 2 Fatigue limit , 1,000 lb/in 2 Cast iron Malleable iron Cast steel Armco iron Plain carbon steels SAE 6150, heat-treated Nitralloy Brasses, various Zirconium crystal bar 20 – 50 50 60 – 80 44 60 – 150 200 125 25 – 75 52 6 – 18 24 24 – 32 24 25 – 75 80 80 7 – 20 16 – 18 NOTE: Stress, 1,000 lb/in 2 ϫ 6.894 ϭ stress, MN/m 2. Metal Tensile strength, 1,000 lb/in 2 Fatigue limit , 1,000 lb/in 2 Copper Monel Phosphor bronze Tobin bronze, hard Cast aluminum alloys Wrought aluminum alloys Magnesium alloys Molybdenum, as cast Titanium (Ti-75A) 32 – 50 70 – 120 55 65 18 – 40 25 – 70 20 – 45 98 91 12 – 17 20 – 50 12 21 6 – 11 8 – 18 7 – 17 45 45
- 10. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-10 MECHANICAL PROPERTIES OF MATERIALS of Cyclic-Thermal Stresses in a Ductile Material, Trans. ASME, 76, 1954, p. 947.) The type of physical change occurring inside a material as it is repeatedly loaded to failure varies as the life is consumed, and a number of stages in fatigue can be distinguished on this basis. The early stages comprise the events causing nucleation of a crack or ﬂaw. This is most likely to appear on the surface of the material; fatigue failures generally originate at a surface. Following nucleation of the crack, it grows during the crack-propagation stage. Eventually the crack becomes large enough for some rapid terminal mode of failure to take over such as ductile rupture or brittle fracture. The rate of crack growth in the crackpropagation stage can be accurately quantiﬁed by fracture mechanics methods. Assuming an initial ﬂaw and a loading situation as shown in Fig. 5.1.15, the rate of crack growth per cycle can generally be expressed as da/dN ϭ C0(⌬KI)n (5.1.3) where C0 and n are constants for a particular material and ⌬KI is the range of stress intensity per cycle. KI is given by (5.1.1). Using (5.1.3), it is possible to predict the number of cycles for the crack to grow to a size at which some other mode of failure can take over. Values of the constants C0 and n are determined from specimens of the same type as those used for determination of KIc but are instrumented for accurate measurement of slow crack growth. Constant-amplitude fatigue-test data are relevant to many rotarymachinery situations where constant cyclic loads are encountered. There are important situations where the component undergoes variable loads and where it may be advisable to use random-load testing. In this method, the load spectrum which the component will experience in service is determined and is applied to the test specimen artiﬁcially. curve OA in Fig. 5.1.19 is the region of primary creep, AB the region of secondary creep, and BC that of tertiary creep. The strain rates, or the slopes of the curve, are decreasing, constant, and increasing, respectively, in these three regions. Since the period of the creep test is usually much shorter than the duration of the part in service, various extrapolation procedures are followed (see Gittus, ‘‘Creep, Viscoelasticity and Creep Fracture in Solids,’’ Wiley, 1975). See Table 5.1.6. In practical applications the region of constant-strain rate (secondary creep) is often used to estimate the probable deformation throughout the life of the part. It is thus assumed that this rate will remain constant during periods beyond the range of the test-data. The working stress is chosen so that this total deformation will not be excessive. An arbitrary creep strength, which is deﬁned as the stress which at a given temperature will result in 1 percent deformation in 100,000 h, has received a certain amount of recognition, but it is advisable to determine the proper stress for each individual case from diagrams of stress vs. creep rate (Fig. 5.1.20) (see ‘‘Creep Data,’’ ASTM and ASME). CREEP Experience has shown that, for the design of equipment subjected to sustained loading at elevated temperatures, little reliance can be placed on the usual short-time tensile properties of metals at those temperatures. Under the application of a constant load it has been found that materials, both metallic and nonmetallic, show a gradual ﬂow or creep even for stresses below the proportional limit at elevated temperatures. Similar effects are present in low-melting metals such as lead at room temperature. The deformation which can be permitted in the satisfactory operation of most high-temperature equipment is limited. In metals, creep is a plastic deformation caused by slip occurring along crystallographic directions in the individual crystals, together with some ﬂow of the grain-boundary material. After complete release of load, a small fraction of this plastic deformation is recovered with time. Most of the ﬂow is nonrecoverable for metals. Since the early creep experiments, many different types of tests have come into use. The most common are the long-time creep test under constant tensile load and the stress-rupture test. Other special forms are the stress-relaxation test and the constant-strain-rate test. The long-time creep test is conducted by applying a dead weight to one end of a lever system, the other end being attached to the specimen surrounded by a furnace and held at constant temperature. The axial deformation is read periodically throughout the test and a curve is plotted of the strain 0 as a function of time t (Fig. 5.1.19). This is repeated for various loads at the same testing temperature. The portion of the Fig. 5.1.19. Typical creep curve. Fig. 5.1.20. Creep rates for 0.35% C steel. Additional temperatures (°F) and stresses (in 1,000 lb/in2) for stated creep rates (percent per 1,000 h) for wrought nonferrous metals are as follows: 60-40 Brass: Rate 0.1, temp. 350 (400), stress 8 (2); rate 0.01, temp 300 (350) [400], stress 10 (3) [1]. Phosphor bronze: Rate 0.1, temp 400 (550) [700] [800], stress 15 (6) [4] [4]; rate 0.01, temp 400 (550) [700], stress 8 (4) [2]. Nickel: Rate 0.1, temp 800 (1000), stress 20 (10). 70 CU, 30 NI. Rate 0.1, temp 600 (750), stress 28 (13 – 18); rate 0.01, temp 600 (750), stress 14 (8 – 9). Aluminum alloy 17 S (Duralumin): Rate 0.1, temp 300 (500) [600], stress 22 (5) [1.5]. Lead pure (commercial) (0.03 percent Ca): At 110°F, for rate 0.1 percent the stress range, lb/in2, is 150 – 180 (60 – 140) [200 – 220]; for rate of 0.01 percent, 50 – 90 (10 – 50) [110 – 150]. Stress, 1,000 lb/in2 ϫ 6.894 ϭ stress, MN/m2, tk ϭ 5⁄9(tF ϩ 459.67). Structural changes may occur during a creep test, thus altering the metallurgical condition of the metal. In some cases, premature rupture appears at a low fracture strain in a normally ductile metal, indicating that the material has become embrittled. This is a very insidious condition and difﬁcult to predict. The stress-rupture test is well adapted to study this effect. It is conducted by applying a constant load to the specimen in the same manner as for the long-time creep test. The nominal stress is then plotted vs. the time for fracture at constant temperature on a log-log scale (Fig. 5.1.21).
- 11. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. CREEP Table 5.1.6 5-11 Stresses for Given Creep Rates and Temperatures* Creep rate 0.1% per 1,000 h Material Temp, °F Creep rate 0.01% per 1,000 h 800 900 1,000 1,100 1,200 800 900 1,000 1,100 1,200 17 – 27 26 – 33 22 27 – 33 8 – 25 7 25 – 35 20 – 40 7 – 10 30 30 11 – 18 18 – 25 15 – 18 20 – 25 5 – 15 2–7 2–6 3–6 4–7 2 1 1–2 2–3 1–2 1 3 3–4 10 – 18 16 – 24 14 – 17 19 – 28 5 – 15 5 20 – 30 8 – 20 3–8 6 – 14 11 – 22 11 – 15 12 – 19 3–7 1 1–2 1 2–5 1–2 35 25 6 – 11 10 – 18 12 3–8 4 – 12 4–7 3–8 2–4 2 3 – 12 1–6 1–2 3–5 2–7 7 – 12 6 1 2 2–3 2–4 1 10 – 20 10 – 15 18 27 3 – 12 9 – 16 9 – 11 7 – 15 5 4 8 – 20 2 – 12 5–4 7 – 10 4 – 10 10 – 15 12 30 – 40 7 – 12 30 30 20 – 70 12 – 20 5 12 21 14 – 30 4 – 14 2 4 6 – 15 5 – 15 25 – 28 8 – 15 2–8 7 30 18 – 50 6 11 8 – 18 1 3–9 2 – 13 1 Temp, °F 1,100 1,200 1,300 1,400 1,500 1,000 1,100 1,200 1,300 1,400 Wrought chrome-nickel steels: 18-8† 10 – 25 Cr, 10 – 30 Ni‡ 10 – 18 10 – 20 5 – 11 5 – 15 3 – 10 3 – 10 2–5 2–5 2.5 11 – 16 5 – 12 6 – 15 2 – 10 3 – 10 2–8 1–2 1–3 800 900 1,000 1,100 1,200 800 900 1,000 1,100 1,200 10 – 20 28 25 – 30 5 – 10 20 – 30 15 – 25 3 6 – 12 8 – 15 20 – 25 4 9 8 – 15 20 20 – 25 10 – 15 9 – 15 1 2–5 2–7 20 2 3 2 15 8 Wrought steels: SAE 1015 0.20 C, 0.50 Mo 0.10 – 0.25 C, 4 – 6 Cr ϩ Mo SAE 4140 SAE 1030 – 1045 Commercially pure iron 0.15 C, 1 – 2.5 Cr, 0.50 Mo SAE 4340 SAE X3140 0.20 C, 4 – 6 Cr 0.25 C, 4 – 6 Cr ϩ W 0.16 C, 1.2 Cu 0.20 C, 1 Mo 0.10 – 0.40 C, 0.2 – 0.5 Mo, 1 – 2 Mn SAE 2340 SAE 6140 SAE 7240 Cr ϩ Va ϩ W, various Temp, °F Cast steels: 0.20 – 0.40 C 0.10 – 0.30 C, 0.5 – 1 Mo 0.15 – 0.30 C, 4 – 6 Cr ϩ Mo 18 – 8§ Cast iron Cr Ni cast iron 20 18 – 28 15 – 30 8 6–8 1–3 1 2–8 3 1 2 2 8 15 12 – 18 10 10 0.5 * Based on 1,000-h tests. Stresses in 1,000 lb/in2. † Additional data. At creep rate 0.1 percent and 1,000 (1,600)°F the stress is 18 – 25 (1); at creep rate 0.01 percent at 1,500°F, the stress is 0.5. ‡ Additional data. At creep rate 0.1 percent and 1,000 (1,600)°F the stress is 10 – 30 (1). § Additional data. At creep rate 0.1 percent and 1,600°F the stress is 3; at creep rate 0.01 and 1,500°F, the stress is 2 – 3. The stress reaction is measured in the constant-strain-rate test while the specimen is deformed at a constant strain rate. In the relaxation test, the decrease of stress with time is measured while the total strain (elastic ϩ plastic) is maintained constant. The latter test has direct application to the loosening of turbine bolts and to similar problems. Although some correlation has been indicated between the results of these various types of tests, no general correlation is yet available, and it has been found necessary to make tests under each of these special conditions to obtain satisfactory results. The interrelationship between strain rate and temperature in the form of a velocity-modiﬁed temperature (see MacGregor and Fisher, A Velocity-modiﬁed Temperature for the Plastic Flow of Metals, Jour. Appl. Mech., Mar. 1945) simpliﬁes the creep problem in reducing the number of variables. Superplasticity Superplasticity is the property of some metals and alloys which permits extremely large, uniform deformation at elevated temperature, in contrast to conventional metals which neck down and subsequently fracture after relatively small amounts of plastic deformation. Superplastic behavior requires a metal with small equiaxed grains, a slow and steady rate of deformation (strain Fig. 5.1.21 Relation between time to failure and stress for a 3% chromium steel. (1) Heat treated 2 h at 1,740°F (950°C) and furnace cooled; (2) hot rolled and annealed 1,580°F (860°C).
- 12. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-12 MECHANICAL PROPERTIES OF MATERIALS rate), and a temperature elevated to somewhat more than half the melting point. With such metals, large plastic deformation can be brought about with lower external loads; ultimately, that allows the use of lighter fabricating equipment and facilitates production of ﬁnished parts to near-net shape. ⌱ ⌱⌱ BHN ϭ P 1.0 ⌱⌱⌱ ⌬ᐉ ␣ ⌬ᐉ ⑀• m ϭ tan ␣ ϭ ⌬ᐉ ր⌬ᐉ ⑀ m In ϭ ⌲⑀• m 0.5 ؋ m • In ⑀• (a) known load into the surface of a material and measuring the diameter of the indentation left after the test. The Brinell hardness number, or simply the Brinell number, is obtained by dividing the load used, in kilograms, by the actual surface area of the indentation, in square millimeters. The result is a pressure, but the units are rarely stated. 0 In ⑀• (b) Fig. 5.1.22. Stress and strain rate relations for superplastic alloys. (a) Log-log plot of ϭ K m; (b) m as a function of strain rate. Stress and strain rates are related for a metal exhibiting superplasticity. A factor in this behavior stems from the relationship between the applied stress and strain rates. This factor m — the strain rate sensitivity index — is evaluated from the equation ϭ K m, where is the applied stress, K is a constant, and is the strain rate. Figure 5.1.22a plots a stress/strain rate curve for a superplastic alloy on log-log coordinates. The slope of the curve deﬁnes m, which is maximum at the point of inﬂection. Figure 5.1.22b shows the variation of m versus ln . Ordinary metals exhibit low values of m — 0.2 or less; for those behaving superplastically, m ϭ 0.6 to 0.8 ϩ. As m approaches 1, the behavior of the metal will be quite similar to that of a newtonian viscous solid, which elongates plastically without necking down. In Fig. 5.1.22a, in region I, the stress and strain rates are low and creep is predominantly a result of diffusion. In region III, the stress and strain rates are highest and creep is mainly the result of dislocation and slip mechanisms. In region II, where superplasticity is observed, creep is governed predominantly by grain boundary sliding. HARDNESS Hardness has been variously deﬁned as resistance to local penetration, to scratching, to machining, to wear or abrasion, and to yielding. The multiplicity of deﬁnitions, and corresponding multiplicity of hardnessmeasuring instruments, together with the lack of a fundamental deﬁnition, indicates that hardness may not be a fundamental property of a material but rather a composite one including yield strength, work hardening, true tensile strength, modulus of elasticity, and others. Scratch hardness is measured by Mohs scale of minerals (Sec. 1.2) which is so arranged that each mineral will scratch the mineral of the next lower number. In recent mineralogical work and in certain microscopic metallurgical work, jeweled scratching points either with a set load or else loaded to give a set width of scratch have been used. Hardness in its relation to machinability and to wear and abrasion is generally dealt with in direct machining or wear tests, and little attempt is made to separate hardness itself, as a numerically expressed quantity, from the results of such tests. The resistance to localized penetration, or indentation hardness, is widely used industrially as a measure of hardness, and indirectly as an indicator of other desired properties in a manufactured product. The indentation tests described below are essentially nondestructive, and in most applications may be considered nonmarring, so that they may be applied to each piece produced; and through the empirical relationships of hardness to such properties as tensile strength, fatigue strength, and impact strength, pieces likely to be deﬁcient in the latter properties may be detected and rejected. Brinell hardness is determined by forcing a hardened sphere under a Ͳͫ ͬ D (D Ϫ √D2 Ϫ d 2) 2 where BHN is the Brinell hardness number; P the imposed load, kg; D the diameter of the spherical indenter, mm; and d the diameter of the resulting impression, mm. Hardened-steel bearing balls may be used for hardness up to 450, but beyond this hardness specially treated steel balls or jewels should be used to avoid ﬂattening the indenter. The standard-size ball is 10 mm and the standard loads 3,000, 1,500, and 500 kg, with 100, 125, and 250 kg sometimes used for softer materials. If for special reasons any other size of ball is used, the load should be adjusted approximately as follows: for iron and steel, P ϭ 30D2; for brass, bronze, and other soft metals, P ϭ 5D2; for extremely soft metals, P ϭ D2 (see ‘‘Methods of Brinell Hardness Testing,’’ ASTM). Readings obtained with other than the standard ball and loadings should have the load and ball size appended, as such readings are only approximately equal to those obtained under standard conditions. The size of the specimen should be sufﬁcient to ensure that no part of the plastic ﬂow around the impression reaches a free surface, and in no case should the thickness be less than 10 times the depth of the impression. The load should be applied steadily and should remain on for at least 15 s in the case of ferrous materials and 30 s in the case of most nonferrous materials. Longer periods may be necessary on certain soft materials that exhibit creep at room temperature. In testing thin materials, it is not permissible to pile up several thicknesses of material under the indenter, as the readings so obtained will invariably be lower than the true readings. With such materials, smaller indenters and loads, or different methods of hardness testing, are necessary. In the standard Brinell test, the diameter of the impression is measured with a low-power hand microscope, but for production work several testing machines are available which automatically measure the depth of the impression and from this give readings of hardness. Such machines should be calibrated frequently on test blocks of known hardness. In the Rockwell method of hardness testing, the depth of penetration of an indenter under certain arbitrary conditions of test is determined. The indenter may be either a steel ball of some speciﬁed diameter or a spherical-tipped conical diamond of 120° angle and 0.2-mm tip radius, called a ‘‘Brale.’’ A minor load of 10 kg is ﬁrst applied which causes an initial penetration and holds the indenter in place. Under this condition, the dial is set to zero and the major load applied. The values of the latter are 60, 100, or 150 kg. Upon removal of the major load, the reading is taken while the minor load is still on. The hardness number may then be read directly from the scale which measures penetration, and this scale is so arranged that soft materials with deep penetration give low hardness numbers. A variety of combinations of indenter and major load are possible; the most commonly used are RB using as indenter a 1⁄16-in ball and a major load of 100 kg and RC using a Brale as indenter and a major load of 150 kg (see ‘‘Rockwell Hardness and Rockwell Superﬁcial Hardness of Metallic Materials,’’ ASTM). Compared with the Brinell test, the Rockwell method makes a smaller indentation, may be used on thinner material, and is more rapid, since hardness numbers are read directly and need not be calculated. However, the Brinell test may be made without special apparatus and is somewhat more widely recognized for laboratory use. There is also a Rockwell superﬁcial hardness test similar to the regular Rockwell, except that the indentation is much shallower. The Vickers method of hardness testing is similar in principle to the Brinell in that it expresses the result in terms of the pressure under the indenter and uses the same units, kilograms per square millimeter. The indenter is a diamond in the form of a square pyramid with an apical
- 13. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. TESTING OF MATERIALS angle of 136°, the loads are much lighter, varying between 1 and 120 kg, and the impression is measured by means of a medium-power compound microscope. V ϭ P/(0.5393d 2) where V is the Vickers hardness number, sometimes called the diamondpyramid hardness (DPH); P the imposed load, kg; and d the diagonal of indentation, mm. The Vickers method is more ﬂexible and is considered to be more accurate than either the Brinell or the Rockwell, but the equipment is more expensive than either of the others and the Rockwell is somewhat faster in production work. Among the other hardness methods may be mentioned the Scleroscope, in which a diamond-tipped ‘‘hammer’’ is dropped on the surface and the rebound taken as an index of hardness. This type of apparatus is seriously affected by the resilience as well as the hardness of the material and has largely been superseded by other methods. In the Monotron method, a penetrator is forced into the material to a predetermined depth and the load required is taken as the indirect measure of the hardness. This is the reverse of the Rockwell method in principle, but the loads and indentations are smaller than those of the latter. In the Herbert pendulum, a 1-mm steel or jewel ball resting on the surface to be tested acts as the fulcrum for a 4-kg compound pendulum of 10-s period. The swinging of the pendulum causes a rolling indentation in the material, and from the behavior of the pendulum several factors in hardness, such as work hardenability, may be determined which are not revealed by other methods. Although the Herbert results are of considerable signiﬁcance, the instrument is suitable for laboratory use only (see Herbert, The Pendulum Hardness Tester, and Some Recent Developments in Hardness Testing, Engineer, 135, 1923, pp. 390, 686). In the Herbert cloudburst test, a shower of steel balls, dropped from a predetermined height, dulls the surface of a hardened part in proportion to its softness and thus reveals defective areas. A variety of mutual indentation methods, in which crossed cylinders or prisms of the material to be tested are forced together, give results comparable with the Brinell test. These are particularly useful on wires and on materials at high temperatures. The relation among the scales of the various hardness methods is not exact, since no two measure exactly the same sort of hardness, and a relationship determined on steels of different hardnesses will be found only approximately true with other materials. The Vickers-Brinell relation is nearly linear up to at least 400, with the Vickers approximately 5 percent higher than the Brinell (actual values run from ϩ 2 to ϩ 11 percent) and nearly independent of the material. Beyond 500, the values become more widely divergent owing to the ﬂattening of the Brinell ball. The Brinell-Rockwell relation is fairly satisfactory and is shown in Fig. 5.1.23. Approximate relations for the Shore Scleroscope are also given on the same plot. The hardness of wood is deﬁned by the ASTM as the load in pounds required to force a ball 0.444 in in diameter into the wood to a depth of 0.222 in, the speed of penetration being 1⁄4 in/min. For a summary Fig. 5.1.23. Hardness scales. 5-13 of the work in hardness see Williams, ‘‘Hardness and Hardness Measurements,’’ ASM. TESTING OF MATERIALS Testing Machines Machines for the mechanical testing of materials usually contain elements (1) for gripping the specimen, (2) for deforming it, and (3) for measuring the load required in performing the deformation. Some machines (ductility testers) omit the measurement of load and substitute a measurement of deformation, whereas other machines include the measurement of both load and deformation through apparatus either integral with the testing machine (stress-strain recorders) or auxiliary to it (strain gages). In most general-purpose testing machines, the deformation is controlled as the independent variable and the resulting load measured, and in many special-purpose machines, particularly those for light loads, the load is controlled and the resulting deformation is measured. Special features may include those for constant rate of loading (pacing disks), for constant rate of straining, for constant load maintenance, and for cyclical load variation (fatigue). In modern testing systems, the load and deformation measurements are made with load-and-deformation-sensitive transducers which generate electrical outputs. These outputs are converted to load and deformation readings by means of appropriate electronic circuitry. The readings are commonly displayed automatically on a recorder chart or digital meter, or they are read into a computer. The transducer outputs are typically used also as feedback signals to control the test mode (constant loading, constant extension, or constant strain rate). The load transducer is usually a load cell attached to the test machine frame, with electrical output to a bridge circuit and ampliﬁer. The load cell operation depends on change of electrical resistivity with deformation (and load) in the transducer element. The deformation transducer is generally an extensometer clipped on to the test specimen gage length, and operates on the same principle as the load cell transducer: the change in electrical resistance in the specimen gage length is sensed as the specimen deforms. Optical extensometers are also available which do not make physical contact with the specimen. Veriﬁcation and classiﬁcation of extensometers is controlled by ASTM Standards. The application of load and deformation to the specimen is usually by means of a screw-driven mechanism, but it may also be applied by means of hydraulic and servohydraulic systems. In each case the load application system responds to control inputs from the load and deformation transducers. Important features in test machine design are the methods used for reducing friction, wear, and backlash. In older testing machines, test loads were determined from the machine itself (e.g., a pressure reading from the machine hydraulic pressure) so that machine friction made an important contribution to inaccuracy. The use of machine-independent transducers in modern testing has eliminated much of this source of error. Grips should not only hold the test specimen against slippage but should also apply the load in the desired manner. Centering of the load is of great importance in compression testing, and should not be neglected in tension testing if the material is brittle. Figure 5.1.24 shows the theoretical errors due to off-center loading; the results are directly applicable to compression tests using swivel loading blocks. Swivel (ball-and-socket) holders or compression blocks should be used with all except the most ductile materials, and in compression testing of brittle materials (concrete, stone, brick), any rough faces should be smoothly capped with plaster of paris and one-third portland cement. Serrated grips may be used to hold ductile materials or the shanks of other holders in tension; a taper of 1 in 6 on the wedge faces gives a self-tightening action without excessive jamming. Ropes are ordinarily held by wet eye splices, but braided ropes or small cords may be given several turns over a ﬁxed pin and then clamped. Wire ropes should be zinced into forged sockets (solder and lead have insufﬁcient strength). Grip selection for tensile testing is described in ASTM standards. Accuracy and Calibration ASTM standards require that commercial machines have errors of less than 1 percent within the ‘‘loading range’’ when checked against acceptable standards of comparison at at least ﬁve suitably spaced loads. The ‘‘loading range’’ may be any range
- 14. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-14 MECHANICS OF MATERIALS through which the preceding requirements for accuracy are satisﬁed, except that it shall not extend below 100 times the least load to which the machine will respond or which can be read on the indicator. The use of calibration plots or tables to correct the results of an otherwise inaccurate machine is not permitted under any circumstances. Machines with errors less than 0.1 percent are commercially available (TateEmery and others), and somewhat greater accuracy is possible in the most reﬁned research apparatus. Two standard forms of test specimens (ASTM) are shown in Figs. 5.1.25 and 5.1.26. In wrought materials, and particularly in those which Fig. 5.1.25. Test specimen, 2-in (50-mm) gage length, 1⁄2-in (12.5-mm) diameter. Others available for 0.35-in (8.75-mm) and 0.25-in (6.25-mm) diameters. (ASTM). Fig. 5.1.26. Charpy V-notch impact specimens. (ASTM.) Fig. 5.1.24. Effect of centering errors on brittle test specimens. Dead loads may be used to check machines of low capacity; accurately calibrated proving levers may be used to extend the range of available weights. Various elastic devices (such as the Morehouse proving ring) made of specially treated steel, with sensitive disortion-measuring devices, and calibrated by dead weights at the NIST (formerly Bureau of Standards) are mong the most satisfactory means of checking the higher loads. 5.2 have been cold-worked, different properties may be expected in different directions with respect to the direction of the applied work, and the test specimen should be cut out from the parent material in such a way as to give the strength in the desired direction. With the exception of fatigue specimens and specimens of extremely brittle materials, surface ﬁnish is of little practical importance, although extreme roughness tends to decrease the ultimate elongation. MECHANICS OF MATERIALS by J. P. Vidosic REFERENCES: Timoshenko and MacCullough, ‘‘Elements of Strength of Materials,’’ Van Nostrand. Seeley, ‘‘Advanced Mechanics of Materials,’’ Wiley. Timoshenko and Goodier, ‘‘Theory of Elasticity,’’ McGraw-Hill. Phillips, ‘‘Introduction to Plasticity,’’ Ronald. Van Den Broek, ‘‘Theory of Limit Design,’’ Wiley. Het´ nyi, ‘‘Handbook of Experimental Stress Analysis,’’ Wiley. Dean and Douge las, ‘‘Semi-Conductor and Conventional Strain Gages,’’ Academic. Robertson and Harvey, ‘‘The Engineering Uses of Holography,’’ University Printing House, London. Sellers, ‘‘Basic Training Guide to the New Metrics and SI Units,’’ National Tool, Die and Precision Machining Association. Roark and Young, ‘‘Formulas for Stress and Strain,’’ McGraw-Hill. Perry and Lissner, ‘‘The Strain Gage Primer,’’ McGraw-Hill. Donnell, ‘‘Beams, Plates, and Sheets,’’ Engineering Societies Monographs, McGraw-Hill. Griffel, ‘‘Beam Formulas’’ and ‘‘Plate Formulas,’’ Ungar. Durelli et al., ‘‘Introduction to the Theoretical and Experimental Analysis of Stress and Strain,’’ McGraw-Hill. ‘‘Stress Analysis Manual,’’ Department of Commerce, Pub. no. AD 759 199, 1969. Blodgett , ‘‘Welded Struc- tures,’’ Lincoln Arc Welding Foundation. ‘‘Characteristics and Applications of Resistance Strain Gages,’’ Department of Commerce, NBS Circ. 528, 1954. EDITOR’S NOTE: The almost universal availability and utilization of computers in engineering practice has led to the development of many forms of software individually tailored to the solution of speciﬁc design problems in the area of mechanics of materials. Their use will permit the reader to amplify and supplement a good portion of the formulary and tabular collection in this section, as well as utilize those powerful computational tools in newer and more powerful techniques to facilitate solutions to problems. Many of the approximate methods, involving laborious iterative mathematical schemes, have been supplanted by the computer. Developments along those lines continue apace and bid fair to expand the types of problems handled, all with greater conﬁdence in the results obtained thereby.
- 15. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. SIMPLE STRESSES AND STRAINS Main Symbols Unit Stress S ϭ apparent stress Sv or Ss ϭ pure shearing T ϭ true (ideal) stress Sp ϭ proportional elastic limit Sy ϭ yield point SM ϭ ultimate strength, tension Sc ϭ ultimate compression Sv ϭ vertical shear in beams SR ϭ modulus of rupture 5-15 parafﬁn; Ϸ 0 for cork. For concrete, varies from 0.10 to 0.20 at working stresses and can reach 0.25 at higher stresses; for ordinary glass is about 0.25. In the absence of deﬁnitive data, for most structural metals can be taken to lie between 0.25 and 0.35. Extensive listings of Poisson’s ratio are found in other sections; see Tables 5.1.3 and 6.1.9. Moment M ϭ bending Mt ϭ torsion External Action P ϭ force G ϭ weight of body W ϭ weight of load V ϭ external shear Fig. 5.2.1 Modulus of Elasticity E ϭ longitudinal G ϭ shearing K ϭ bulk Up ϭ modulus of resilience UR ϭ ultimate resilience Stress is an internal distributed force, or, force per unit area; it is the internal mechanical reaction of the material accompanying deformation. Stresses always occur in pairs. Stresses are normal [tensile stress (ϩ) and compressive stress (Ϫ)]; and tangential, or shearing. Geometric l ϭ length A ϭ area V ϭ volume v ϭ velocity r ϭ radius of gyration I ϭ rectangular moment of inertia IP or J ϭ polar moment of inertia Deformation e, eЈ ϭ gross deformation , Ј ϭ unit deformation; strain d or ␣ ϭ unit, angular sЈ ϭ unit, lateral ϭ Poisson’s ratio n ϭ reciprocal of Poisson’s ratio r ϭ radius f ϭ deﬂection SIMPLE STRESSES AND STRAINS Deformations are changes in form produced by external forces or loads that act on nonrigid bodies. Deformations are longitudinal, e, a lengthening (ϩ) or shortening (Ϫ) of the body; and angular, ␣, a change of angle between the faces. Unit deformation (dimensionless number) is the deformation in unit distance. Unit longitudinal deformation (longitudinal strain), ϭ e/l (Fig. 5.2.1). Unit angular-deformation tan ␣ equals ␣ approx (Fig. 5.2.2). The accompanying lateral deformation results in unit lateral deformation (lateral strain) Ј ϭ eЈ/lЈ (Fig. 5.2.1). For homogeneous, isotropic material operating in the elastic region, the ratio Ј/ is a constant and is a deﬁnite property of the material; this ratio is called Poisson’s ratio . A fundamental relation among the three interdependent constants E, G, and for a given material is E ϭ 2G(1 ϩ ). Note that cannot be larger than 0.5; thus the shearing modulus G is always smaller than the elastic modulus E. At the extremes, for example, Ϸ 0.5 for rubber and Fig. 5.2.2 Intensity of stress, or unit stress, S, lb/in2 (kgf/cm2), is the amount of force per unit of area (Fig. 5.2.3). P is the load acting through the center of gravity of the area. The uniformly distributed normal stress is S ϭ P/A When the stress is not uniformly distributed, S ϭ dP/dA. A long rod will stretch under its own weight G and a terminal load P (see Fig. 5.2.4). The total elongation e is that due to the terminal load plus that due to one-half the weight of the rod considered as acting at the end. e ϭ (Pl ϩ Gl/2)/(AE) The maximum stress is at the upper end. When a load is carried by several paths to a support, the different paths take portions of the load in proportion to their stiffness, which is controlled by material (E) and by design. EXAMPLE. Two pairs of bars rigidly connected (with the same elongation) carry a load P0 (Fig. 5.2.5). A1 , A2 and E1 , E2 and P1 , P2 and S1 , S2 are cross sections, moduli of elasticity, loads, and stresses of the bars, respectively; e ϭ elongation. e ϭ P1l(E1A1) ϭ P2 l/(E2 A2) P0 ϭ 2P1 ϩ 2P2 S2 ϭ P2 /A2 ϭ 1⁄2[P0 E2 /(E1 A1 ϩ E2 A2)] S1 ϭ 1⁄2[P0 E1 /(E1A1 ϩ E2 A2)] Temperature Stresses When the deformation arising from change of temperature is prevented, temperature stresses arise that are proportional to the amount of deformation that is prevented. Let a ϭ coefﬁ-
- 16. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-16 MECHANICS OF MATERIALS Fig. 5.2.7 Fig. 5.2.3 Fig. 5.2.4 Fig. 5.2.8 and Fig. 5.2.8 a common form of test piece that introduces bending stresses. Let Fig. 5.2.9 represent the symmetric section of area A with a shearing force V acting through its centroid. If pure shear exists, Sv ϭ V/A, and this shear would be uniformly distributed over the area A. When this shear is accompanied by bending (transverse shear in beams), the unit shear cient of expansion per degree of temperature, l1 ϭ length of bar at temperature t1 , and l 2 ϭ length at temperature t2 . Then l 2 ϭ l1[1 ϩ a(t2 Ϫ t1)] If, subsequently, the bar is cooled to a temperature t1 , the proportionate deformation is s ϭ a(t2 Ϫ t1) and the corresponding unit stress S ϭ Ea(t2 Ϫ t1). For coefﬁcients of expansion, see Sec. 4. In the case of steel, a change of temperature of 12°F (6.7 K, 6.7°C) will cause in general a unit stress of 2,340 lb/in2 (164 kgf/cm2). Fig. 5.2.9 Sv increases from the extreme ﬁber to its maximum, which may or may not be at the neutral axis OZ. The unit shear parallel to OZ at a point d distant from the neutral axis (Fig. 5.2.9) is Sv ϭ Fig. 5.2.5 V Ib ͵ e yz dy d where z ϭ the section width at distance y; and I is the moment of inertia of the entire section about the neutral axis OZ. Note that ͐e yz dy is the d ﬁrst moment of the area above d with respect to axis OZ. For a rectangular cross section (Fig. 5.2.10a), Shearing stresses (Fig. 5.2.2) act tangentially to surface of contact and do not change length of sides of elementary volume; they change the angle between faces and the length of diagonal. Two pairs of shearing stresses must act together. Shearing stress intensities are of equal magnitude on all four faces of an element. Sv ϭ SЈ (Fig. 5.2.6). v 3 2 3 Sv (max) ϭ 2 Sv ϭ ͫ ͩ ͪͬ V 1Ϫ bh V 3 V ϭ bh 2 A 2y h 2 for y ϭ 0 For a circular cross section (Fig. 5.2.10b), 4 3 4 Sv (max) ϭ 3 Sv ϭ Fig. 5.2.6 In the presence of pure shear on external faces (Fig. 5.2.6), the resultant stress S on one diagonal plane at 45° is pure tension and on the other diagonal plane pure compression; S ϭ Sv ϭ SЈ . S on diagonal plane is v called ‘‘diagonal tension’’ by writers on reinforced concrete. Failure under pure shear is difﬁcult to produce experimentally, except under torsion and in certain special cases. Figure 5.2.7 shows an ideal case, Fig. 5.2.10 ͫ ͩ ͪͬ V 1Ϫ r2 4 V V ϭ r2 3 A y r 2 for y ϭ 0
- 17. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. SIMPLE STRESSES AND STRAINS 5-17 Table 5.2.1 Resilience per Unit of Volume Up (S ϭ longitudinal stress; Sv ϭ shearing stress; E ϭ tension modulus of elasticity; G ϭ shearing modulus of elasticity) Tension or compression Shear Beams (free ends) Rectangular section, bent in arc of circle; no shear Ditto, circular section Concentrated center load; rectangular cross section Ditto, circular cross section Uniform load, rectangular cross section 1-beam section, concentrated center load ⁄ S 2/E ⁄ S 2 /G v 12 12 ⁄ 16 S 2/E S 2/E ⁄ ⁄ S 2/E 18 1 18 ⁄ S 2/E ⁄ S 2/E 3⁄32S 2/E 1 24 5 36 For a circular ring (thickness small in comparison with the major diameter), Sv(max) ϭ 2V/A, for y ϭ 0. For a square cross section (diagonal vertical, Fig. 5.2.10c), Sv ϭ V √2 a2 ͫ Sv (max) ϭ 1.591 1ϩ V A ͩ ͪͬ y √2 y Ϫ4 a a e for y ϭ 4 2 For an I-shaped cross section (Fig. 5.2.10d), Sv (max) ϭ 3 V 4 a ͫ be 2 Ϫ (b Ϫ a)f 2 be 3 Ϫ (b Ϫ a)f 3 ͬ for y ϭ 0 Elasticity is the ability of a material to return to its original dimensions after the removal of stresses. The elastic limit Sp is the limit of stress within which the deformation completely disappears after the removal of stress; i.e., no set remains. Hooke’s law states that, within the elastic limit, deformation produced is proportional to the stress. Unless modiﬁed, the deduced formulas of mechanics apply only within the elastic limit. Beyond this, they are modiﬁed by experimental coefﬁcients, as, for instance, the modulus of rupture. The modulus of elasticity, lb/in2 (kgf/cm2), is the ratio of the increment of unit stress to increment of unit deformation within the elastic limit. The modulus of elasticity in tension, or Young’s modulus, E ϭ unit stress/unit deformation ϭ Pl/(Ae) The modulus of elasticity in compression is similarly measured. The modulus of elasticity in shear or coefﬁcient of rigidity, G ϭ Sv /␣ where ␣ is expressed in radians (see Fig. 5.2.2). The bulk modulus of elasticity K is the ratio of normal stress, applied to all six faces of a cube, to the change of volume. Change of volume under normal stress is so small that it is rarely of signiﬁcance. For example, given a body with length l, width b, thickness d, Poisson’s ratio , and longitudinal strain , V ϭ lbd ϭ original volume. The deformed volume ϭ (1 ϩ )l (1 Ϫ )b(1 Ϫ )d. Neglecting powers of , the deformed volume ϭ (1 ϩ Ϫ 2)V. The change in volume is (1 Ϫ 2)V; the unit volumetric strain is (1 Ϫ 2). Thus, a steel rod ( ϭ 0.3, E ϭ 30 ϫ 106 lb/in2) compressed to a stress of 30,000 lb/in2 will experience ϭ 0.001 and a unit volumetric strain of 0.0004, or 1 part in 2,500. The following relationships exist between the modulus of elasticity in tension or compression E, modulus of elasticity in shear G, bulk modulus of elasticity K, and Poisson’s ratio : E ϭ 2G(1 ϩ ) G ϭ E/[2(1 ϩ )] ϭ (E Ϫ 2G)/(2G) K ϭ E/[3(1 Ϫ 2)] ϭ (3K Ϫ E)/(6K) Resilience U (in и lb)[(cm и kgf )] is the potential energy stored up in a deformed body. The amount of resilience is equal to the work required to deform the body from zero stress to stress S. When S does not exceed Torsion Solid circular 14 2 ⁄ S v /G 2 R1 ϩ R2 1 S 2 2 v 2 R1 4 G Hollow, radii R1 and R2 Springs Carriage Flat spiral, rectangular section Helical: axial load, circular wire Helical: axial twist Helical: axial twist , rectangular section ⁄ S 2/E ⁄ S 2/E 1⁄4S 2/G v 1⁄8S 2/E 1⁄6S 2/E 16 1 24 the elastic limit. For normal stress, resilience ϭ work of deformation ϭ average force times deformation ϭ 1⁄2 Pe ϭ 1⁄2 AS ϫ Sl/E ϭ 1⁄2 S 2V/E. Modulus of resilience Up (in и lb/in3) [(cm и kgf/cm3)], or unit resilience, is the elastic energy stored up in a cubic inch of material at the elastic limit. For normal stress, Up ϭ 1⁄2 S 2 /E p The unit resilience for any other kind of stress, as shearing, bending, torsion, is a constant times one-half the square of the stress divided by the appropriate modulus of elasticity. For values, see Table 5.2.1. Unit rupture work UR , sometimes called ultimate resilience, is measured by the area of the stress-deformation diagram to rupture. UR ϭ 1⁄3 eu(Sy ϩ 2SM ) approx where eu is the total deformation at rupture. For structural steel, UR ϭ 1⁄3 ϫ 27⁄100 ϫ [35,000 ϩ (2 ϫ 60,000)] ϭ 13,950 in и lb/in3 (982 cm и kgf/cm3). EXAMPLE 1. A load P ϭ 40,000 lb compresses a wooden block of cross-sectional area A ϭ 10 in2 and length ϭ 10 in, an amount e ϭ 4⁄100 in. Stress S ϭ 1⁄10 ϫ 40,000 ϭ 4,000 lb/in2. Unit elongation s ϭ 4⁄100 Ϭ 10 ϭ 1⁄250. Modulus of elasticity E ϭ 4,000 Ϭ 1⁄250 ϭ 1,000,000 lb/in2. Unit resilience U p ϭ 1⁄2 ϫ 4,000 ϫ 4,000/ 1,000,000 ϭ 8 in и lb/in3 (0.563 cm и kgf/cm3). EXAMPLE 2. A weight G ϭ 5,000 lb falls through a height h ϭ 2 ft; V ϭ number of cubic inches required to absorb the shock without exceeding a stress of 4,000 lb/in2. Neglect compression of block . Work done by falling weight ϭ Gh ϭ 5,000 ϫ 2 ϫ 12 in и lb (2,271 ϫ 61 cm и kgf ) Resilience of block ϭ V ϫ 8 in и lb ϭ 5,000 ϫ 2 ϫ 12. Therefore, V ϭ 15,000 in3 (245,850 cm3). Thermal Stresses A bar will change its length when its temperature is raised (or lowered) by the amount ⌬l 0 ϭ ␣l 0(t2 Ϫ 32). The linear coefﬁcient of thermal expansion ␣ is assumed constant at normal temperatures and l 0 is the length at 32°F (273.2 K, 0°C). If this expansion (or contraction) is prevented, a thermal-time stress is developed, equal to S ϭ E␣(t2 Ϫ t1), as the temperature goes from t1 to t2 . In thin ﬂat plates the stress becomes S ϭ E␣(t2 Ϫ t1)/(1 Ϫ ); is Poisson’s ratio. Such stresses can occur in castings containing large and small sections. Similar stresses also occur when heat ﬂows through members because of the difference in temperature between one point and another. The heat ﬂowing across a length b as a result of a linear drop in temperature ⌬t equals Q ϭ k A⌬t/b Btu/h (cal/h). The thermal conductivity k is in Btu/(h)(ft2)(°F)/(in of thickness) [cal/(h)(m2)(k)/(m)]. The thermal-ﬂow stress is then S ϭ E␣Qb/( kA). Note, when Q is substituted the stress becomes S ϭ E␣ ⌬t as above, only t is now a function of distance rather than time. EXAMPLE. A cast-iron plate 3 ft square and 2 in thick is used as a ﬁre wall. The temperature is 330°F on the hot side and 160°F on the other. What is the thermal-ﬂow stress developed across the plate? or and S ϭ E␣ ⌬t ϭ 13 ϫ 106 ϫ 6.5 ϫ 10Ϫ6 ϫ 170 ϭ 14,360 lb/in2 (1,010 kgf/cm2 ) Q ϭ 2.3 ϫ 9 ϫ 170/ 2 ϭ 1,760 Btu / h S ϭ 13 ϫ 106 ϫ 6.5 ϫ 10Ϫ6 ϫ 1,760 ϫ 2 / 2.3 ϫ 9 ϭ 14,360 lb/in2 (1,010 kgf/cm2 )
- 18. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-18 MECHANICS OF MATERIALS COMBINED STRESSES 60° Sn ϭ In the discussion that follows, the element is subjected to stresses lying in one plane; this is the case of plane stress, or two-dimensional stress. Simple stresses, deﬁned as such by the ﬂexure and torsion theories, lie in planes normal or parallel to the line of action of the forces. Normal, as well as shearing, stresses may, however, exist in other directions. A particle out of a loaded member will contain normal and shearing stresses as shown in Fig. 5.2.11. Note that the four shearing stresses must be of the same magnitude, if equilibrium is to be satisﬁed. If the particle is ‘‘cut’’ along the plane AA, equilibrium will reveal that, in general, normal as well as shearing stresses act upon the plane AC (Fig. 5.2.12). The normal stress on plane AC is labeled Sn , and shearing Ss . The application of equilibrium yields Sx ϩ Sy S Ϫ Sy ϩ x cos 2 ϩ Sxy sin 2 2 2 S Ϫ Sy Ss ϭ x sin 2 Ϫ Sxy cos 2 2 Sn ϭ and Fig. 5.2.11 4,000 ϩ 8,000 4,000 Ϫ 8,000 ϩ (Ϫ 0.5000) ϩ 0 2 2 ϭ 7,000 lb/in2 4,000 Ϫ 8,000 (0.8660) Ϫ 0 ϭ Ϫ 1,732 lb/in2 60° Ss ϭ 2 4,000 ϩ 8,000 4,000 Ϫ 8,000 2 SM,m ϭ ϩ0 Ϯ 2 2 ϭ 6,000 Ϯ 2,000 ϭ 8,000 and 4,000 lb/in2 (564 and 282 kgf/cm2) 2ϫ0 ϭ 0 or ϭ 90° and 0° at tan 2 ϭ 4,000 Ϫ 8,000 4,000 Ϫ 8,000 2 ϩ0 Ss M,m ϭ Ϯ 2 2 (Ϯ 141 kgf/cm2) ϭ Ϯ 2,000 lb/in √ͩ √ͩ ͪ ͪ Mohr’s Stress Circle The biaxial stress ﬁeld with its combined stresses can be represented graphically by the Mohr stress circle. For instance, for the particle given in Fig. 5.2.11, Mohr’s circle is as shown in Fig. 5.2.14. The stress sign convention previously deﬁned must be adhered to. Furthermore, in order to locate the point (on Mohr’s circle) that yields the stresses on a plane ° from the vertical side of the particle (such as plane AA in Fig. 5.2.11), 2° must be laid off in the same Fig. 5.2.12 A sign convention must be used. A tensile stress is positive while compression is negative. A shearing stress is positive when directed as on plane AB of Fig. 5.2.12; i.e., when the shearing stresses on the vertical planes form a clockwise couple, the stress is positive. The planes deﬁned by tan 2 ϭ 2Sxy /Sx Ϫ Sy , the principal planes, contain the principal stresses — the maximum and minimum normal stresses. These stresses are S ϩ Sy Ϯ S M , Sm ϭ x 2 √ͩ Sx Ϫ Sy 2 ͪ 2 ϩ S2 xy The maximum and minimum shearing stresses are represented by the quantity Ss M,m ϭ Ϯ √ͩ Sx Ϫ Sy 2 ͪ 2 Fig. 5.2.14 direction from the radius to (Sx , Sxy ). For the previous example, Mohr’s circle becomes Fig. 5.2.15. Eight special stress ﬁelds are shown in Figs. 5.2.16 to 5.2.23, along with Mohr’s circle for each. ϩ S2 xy and they act on the planes deﬁned by tan 2 ϭ Ϫ Sx Ϫ Sy 2Sxy EXAMPLE. The steam in a boiler subjects a paticular particle on the outer surface of the boiler shell to a circumferential stress of 8,000 lb/in2 and a longitudinal stress of 4,000 lb/in2 as shown in Fig. 5.2.13. Find the stresses acting on the plane XX, making an angle of 60° with the direction of the 8,000 lb/in2 stress. Find the principal stresses and locate the principal planes. Also ﬁnd the maximum and minimum shearing stresses. Fig. 5.2.15 Fig. 5.2.13 Combined Loading Combined ﬂexure and torsion arise, for instance, when a shaft twisted by a torque Mt is bent by forces produced by belts or gears. An element on the surface, such as ABCD on the shaft of Fig. 5.2.24, is subjected to a ﬂexure stress Sx ϭ Mc/I ϭ 8Fl( d 3) and a
- 19. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. PLASTIC DESIGN 5-19 compression) occurring at a point in two right-angle directions, and the change of the angle between them is ␥xy . The strain e at the point in any direction a at an angle with the x direction derives as e Ϫ ey ␥ e ϩ ey ϩ x cos 2 ϩ xy sin 2 ea ϭ x 2 2 2 Fig. 5.2.16 Fig. 5.2.17 Fig. 5.2.18 Fig. 5.2.19 Fig. 5.2.20 Fig. 5.2.21 Fig. 5.2.22 Similarly, the shearing strain ␥ab (change in the original right angle between directions a and b) is deﬁned by ␥ab ϭ (ex Ϫ ey ) sin 2 ϩ ␥xy cos 2 Inspection easily reveals that the above equations for ea and ␥ab are mathematically identical to those for Sn and Ss . Thus, once a sign convention is established, a Mohr circle for strain can be constructed and used as the stress circle is used. The strain e is positive when an extension and negative when a contraction. If the direction associated with the ﬁrst subscript a rotates counterclockwise during straining with respect to the direction indicated by the second subscript b, the shearing strain is positive; if clockwise, it is negative. In constructing the circle, positive extensional strains will be plotted to the right as abscissas and positive half-shearing strains will be plotted upward as ordinates. For the strains shown in Fig. 5.2.26a, Mohr’s strain circle becomes that shown in Fig. 5.2.26b. The extensional strain in the direction a, making an angle of a with the x direction, is ea , and the shearing strain is ␥ab counterclockwise. The strain 90° away is eb . The maximum principal strain is eM at an angle M clockwise from the x direction. The other principal or minimum strain is em 90° away. Fig. 5.2.23 torsional shearing stress Sxy ϭ Mtc/J ϭ 16Mt( d 3). These stresses will induce combined stresses. The maximum combined stresses will be and Sn ϭ 1⁄2 (Sx Ϯ √S 2 ϩ 4S 2 ) x xy Ss ϭ Ϯ 1⁄2 √S 2 ϩ 4S 2 x xy The above situation applies to any case of normal stress with shear, as when a bolt is under both tension and shear. A beam particle subjected to both ﬂexure and transverse shear is another case. Fig. 5.2.26 Fig. 5.2.24 Combined torsion and longitudinal loads exist on a propeller shaft. A particle on this shaft will contain a tensile stress computed using S ϭ F/A and a torsion shearing stress equal to Ss ϭ Mtc/J. The free body of a particle on the surface of a vertical turbine shaft is subjected to direct compression and torsion. Fig. 5.2.25 When combined loading results in stresses of the same type and direction, the addition is algebraic. Such a situation exists on an offset link like that of Fig. 5.2.25. Mohr’s Strain Circle Strain equations can also be derived for planestrain ﬁelds. Strains ex and ey are the extensional strains (tension or PLASTIC DESIGN Early efforts in stress analysis were based on limit loads, that is, loads which stress a member ‘‘wholly’’ to the yield strength. Euler’s famous paper on column action (‘‘Sur la Force des Colonnes,’’ Academie des Sciences de Berlin, 1757) deals with the column problem this way. More recently, the concept of limit loads, referred to as limit, or plastic, design, has found strong application in the design of certain structures. The theory presupposes a ductile material, absence of stress raisers, and fabrication free of embrittlement. Local load overstress is allowed, provided the structure does not deform appreciably. To visualize the limit-load approach, consider a simple beam of uniform section subjected to a concentrated load of midspan, as depicted in Fig. 5.2.27a. According to elastic theory, the outermost ﬁber on each side and at midspan — the section of maximum bending moment — will ﬁrst reach the yield-strength value. Across the depth of the beam, the stress distribution will, of course, follow the triangular pattern, becoming zero at the neutral axis. If the material is ductile, the stress in the outermost ﬁbers will remain at the yield value until every other ﬁber reaches the same value as the load increases. Thus the stress distribution assumes the rectangular pattern before the plastic hinge forms and failure ensues.
- 20. Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5-20 MECHANICS OF MATERIALS The problem is that of ﬁnding the ﬁnal limit load. Elastic-ﬂexure theory gives the maximum load — triangular distribution — as Fy ϭ 2Sy bh 2 3l equal to one-half the moment at either end. A preferable situation, it might be argued, is one in which the moments are the same at the three stations — solid line. Thus, applying equilibrium to, say, the left half of the beam yields a bending moment at each of the three plastic hinges of ML ϭ For the rectangular stress distribution, the limit load becomes FL ϭ Sy bh 2 l The ratio FL /Fy ϭ 1.50 — an increase of 50 percent in load capability. The ratio FL /Fy has been named shape factor (Jenssen, Plastic Design in Welded Structures Promises New Economy and Safety, Welding Jour., Mar. 1959). See Fig. 5.2.27b for shape factors for some other sections. The shape factor may also be determined by dividing the ﬁrst moment of area about the neutral axis by the section modulus. Fig. 5.2.27 A constant-section beam with both ends ﬁxed, supporting a uniformly distributed load, illustrates another application of the plasticload approach. The bending-moment diagram based on the elastic theory drawn in Fig. 5.2.28 (broken line) shows a moment at the center wl 2 16 DESIGN STRESSES If a machine part is to safely transmit loads acting upon it, a permissible maximum stress must be established and used in the design. This is the allowable stress, the working stress, or preferably, the design stress. The design stress should not waste material, yet should be large enough to prevent failure in case loads exceed expected values, or other uncertainties react unfavorably. The design stress is determined by dividing the applicable material property — yield strength, ultimate strength, fatigue strength — by a factor of safety. The factor should be selected only after all uncertainties have been thoroughly considered. Among these are the uncertainty with respect to the magnitude and kind of operating load, the reliability of the material from which the component is made, the assumptions involved in the theories used, the environment in which the equipment might operate, the extent to which localized and fabrication stresses might develop, the uncertainty concerning causes of possible failure, and the endangering of human life in case of failure. Factors of safety vary from industry to industry, being the result of accumulated experience with a class of machines or a kind of environment. Many codes, such as the ASME code for power shafting, recommend design stresses found safe in practice. In general, the ductility of the material determines the property upon which the factor should be based. Materials having an elongation of over 5 percent are considered ductile. In such cases, the factor of safety is based upon the yield strength or the endurance limit. For materials with an elongation under 5 percent, the ultimate strength must be used because these materials are brittle and so fracture without yielding. Factors of safety based on yield are often taken between 1.5 and 4.0. For more reliable materials or well-deﬁned design and operating conditions, the lower factors are appropriate. In the case of untried materials or otherwise uncertain conditions, the larger factors are safer. The same values can be used when loads vary, but in such cases they are applied to the fatigue or endurance strength. When the ultimate strength determines the design stress (in the case of brittle materials), the factors of safety can be doubled. Thus, under static loading, the design stress for, say, SAE 1020, which has a yield strength of 45,000 lb/in2 (3,170 kgf/cm2) may be taken at 45,000/2, or 22,500 lb/in2 (1,585 kgf/cm2), if a reasonably certain design condition exists. A Class 30 cast-iron part might be designed at 30,000/5 or 6,000 lb/in2 (423 kgf/cm2). A 2017S-0 aluminumalloy component (13,000 lb/in2 endurance strength) could be computed at a design stress of 13,000/2.5 or 5,200 lb/in2 (366 kgf/cm2) in the usual fatigue-load application. BEAMS For properties of structural steel and wooden beams, see Sec. 12.2. Notation Fig. 5.2.28 I ϭ rectangular moment of inertia Ip ϭ polar moment of inertia I/c ϭ section modulus M ϭ bending moment P, W Ј ϭ concentrated load Q or V ϭ total vertical shear R ϭ reaction S ϭ unit normal stress Ss or Sv ϭ transverse shearing stress W ϭ total distributed load

No public clipboards found for this slide

Be the first to comment